PART 400 PAVEMENT - Wichita, Kansas Part 400_Pavement.pdf · This work shall result in bringing the...
Embed Size (px)
Transcript of PART 400 PAVEMENT - Wichita, Kansas Part 400_Pavement.pdf · This work shall result in bringing the...
PART 400 PAVEMENT
TABLE OF CONTENTS
SECTION TITLE PAGE(S)
401 Subgrade Preparation. 3-4
402 Lime Treated Subgrade.. 5-8
403 Portland Cement/Fly Ash Treated Subgrade.. 9-14
404 Geogrid Reinforced Aggregate Base 15-18
405 Asphaltic Concrete Pavement 19-30
406 Portland Cement Concrete Pavement.. 31-38
407 Curb, Gutter, Driveway Approaches, Sidewalk and Wheelchair Ramps
408 Concrete Curing and Protection 45-46
409 Cold Milling Pavement 47-48
410 Cold Plastic Traffic Marking 49-52
This page was left blank for future use.
This work shall result in bringing the subgrade under pavement to the proper distance below the grade of
the finished pavement by excavating or filling as necessary and in preparing the subgrade material to
support the proposed pavement. All excavation, preparation and completion of the roadway subgrade,
water and material furnished, mixing, blading, rolling, cleaning, and furnishing tools and labor to complete
this work is included.
401.2 TESTING PROCEDURES
Tests used to determine optimum moisture content and standard density of the various soils shall
conform to the methods set out in the latest revision of ASTM D-698 unless indicated otherwise on the
plans. Tests used to determine optimum moisture content and standard density of the various soils shall
conform to the methods set out in the latest revision of ASTM D-1557 when specified by the plans.
Laboratory determination of moisture content of the various soils shall conform to the latest revisions of
ASTM D-2216. Field determination of the density of the various soils shall conform to any one of the
methods specified in the latest revisions of ASTM D-1556, D-1267, or D-2922. Field determination of the
moisture content of the various soils shall conform to any one of the methods specified in the latest
revisions of ASTM D-2216 or D-3017.
401.3 CONSTRUCTION REQUIREMENTS
The earth below the finished pavement grade in cut sections shall be scarified, broken up and uniformly
mixed for a minimum depth of six inches (6") and for a minimum distance of eight inches (8") beyond the
back of curb lines, adjusted to a uniform moisture content as described in moisture control requirements
(this section), and compacted to a density equal to or greater than ninety-five percent (95%) of standard
density of the soil involved as determined by the Engineer. The top of the finished and compacted
subgrade shall be slightly higher than the bottom elevation of the proposed pavement.
Compacted fill shall be constructed as necessary to bring the subgrade to the proper elevation to support
the pavement, including curb and gutter, by using excavated material for that purpose. The Contractor
shall remove all sod and vegetable matter, all unstable material, and any other unsuitable material, as
determined by the Engineer, from the surface upon which compacted fill is to be placed. The surface
upon which compacted fill is then to be constructed shall be scarified and broken up to minimum depth of
six inches (6"), adjusted to a moisture content of not less than five percentage points below the optimum
moisture content of the soil involved as determined by the Engineer, and then compacted to the density
requirement to which the subsequently placed compacted fill is to be constructed. Compacted fill shall be
constructed of earth free from animal and vegetable matter and shall be deposited in layers of not more
than six inches (6") in compacted thickness. Each layer shall be thoroughly leveled with a motor grader or
bulldozer and completely compacted to the required density using a sheep's foot roller before the
succeeding layer is placed.
Compacted fill shall be constructed to the line established by the bottom of the proposed pavement to a
width of one foot (1') beyond the right-of-way line and then on a one-to-one slope down to the existing
ground, unless otherwise shown on plans. The process of placing six inch (6") layers of earth, adjusting
moisture content, and compacting the layers is to be continued until the surface of the fill is slightly above
the bottom grade of the proposed pavement and to the width previously specified. The top six inch (6")
layer of compacted fill upon which the pavement is to be placed for a width of eight inches (8") wider on
each side of the proposed pavement shall be brought to the previously specified uniform moisture content
and then compacted to a density equal to or greater than ninety-five percent (95%) of standard density of
the soil involved as determined by the Engineer.
Final Compaction and Grading
When cut or fill operations are complete, the subgrade shall be graded to approximately the bottom of the
proposed pavement. Prior to application of any stabilizing agent (if used), the entire subgrade must be
rolled with a flat steel roller weighing not less than eight (8) tons or more than fifteen (15) tons, after which
all unstable areas must be removed and replaced with suitable material, and all other areas that give
under the weight of the roller shall be re-compacted or otherwise secured from settlement. All work
required to stabilize the subgrade prior to the application of any stabilizing agent (if used) shall be at the
contractor's expense. All earthwork must be completed to approximately the proper distance below the
finished grade of the pavement and to the minimum widths specified prior to preceding with the next
phase of construction on the subgrade and the Contractor shall obtain approval from the Engineer before
proceeding with the next phase of construction. The subgrade must then be brought to a true grade
immediately in advance of paving operations, using procedures previously described in this section.
Trenches and Excavation
It shall be the responsibility of the Contractor to insure that all trenches or excavations made in the
subgrade are backfilled properly, adjusted to the required uniform moisture content, and compacted to the
specified density. The top two foot layer of all trenches that have been sand filled and flushed shall
consist of material identical to the surrounding subgrade and shall be compacted in the same manner as
previously specified to the required density. The Engineer shall have full authority to determine the
acceptability of all trench backfill.
Moisture Control Requirements
The moisture content of the soil being compacted shall be considered as being too high to insure
compaction when after repeated rolling with the sheepsfoot roller, the roller continues to pick up
excessive amounts of soil and refuses to "build up" so that the tamping feet eventually ride the compacted
surface. When heavy clay soils are encountered actual moisture content of the soil shall be no more than
two percentage points above the plastic limit of that soil during compaction.
When other types of rollers are used, the moisture content of the soil shall be considered as excessive
when "bridging" or "building up" of the soil occurs in front of, or behind the wheels of such rollers, and/or
when earth hauling equipment produces excessive ruts in the rolled surfaces.
When frozen soil exists in either the surface of the original ground or the surface of a partially constructed
fill, work shall not proceed until such time that the frozen soil has completely thawed or been removed.
Frozen soil shall not be used in constructing compacted fill.
LIME TREATED SUBGRADE
This work consists of incorporating Carbide lime sludge, Hydrated lime or Pebble quicklime, as a
stabilizing agent, into prepared roadway subgrades. Only one type of lime shall be used on each
The available lime index expressed as a percentage by weight of calcium and magnesium oxides (non-
volatile basis) shall be determined by the "Rapid Suger" test as set out in ASTM C-25. The lime supplier
shall certify, in writing that the lime furnished meets the requirements specified below. The City reserves
the right to sample the lime at the construction site and to test it to verify the certification.
Carbide Lime Sludge
Carbide lime sludge samples shall be submitted to the Engineer prior to construction to determine
composition and application rate.
Hydrated lime shall have a chemical composition such that the minimum available lime index shall not be
less than ninety percent (90%). The fineness of the hydrated lime shall be such that not more than five
percent (0.05%) will be retained on a No. 30 sieve or more than twenty percent (20%) will be retained on
a No. 200 sieve.
Pebble quicklime shall have a chemical composition such that the minimum available lime index shall not
be less than ninety percent (90%). The fineness of the pebble quicklime shall be such that one hundred
percent (100%) will pass a 5/8-inch sieve and not less than eighty percent (80%) will be retained on a 1/4-
402.3 SUBGRADE PREPARATION
Prior to the application of the lime, the subgrade shall be prepared as described in Section 401.
No lime shall be applied unless the temperature is at least forty (40) degrees F. in the shade, away from
artificial heat, and rising, unless otherwise directed by the Engineer.
Lime shall be spread on the subgrade in the specified manner and in such a quantity that the required
amount of lime can be incorporated into the subgrade soil. The application rate to be used will be
determined by the Engineer consistent with the various types of subgrade soils. The soil, lime, and water
shall be mixed by approved road mixers or other approved equipment until a uniform mixture is obtained
and all clods and lumps are reduced to a maximum of two and one-half inches (2 1/2") diameter in size.
This mixture shall extend to a depth of six inches (6") and for a distance of eight inches (8") beyond the
back of the curb lines of the pavement, unless indicated otherwise by the plans or contract.
Carbide Sludge Lime
Carbide lime sludge shall be spread using methods that have been approved by the Engineer which will
result in the specified uniform rate of application. Continued use of methods which do not result in a
uniform application will not be permitted. All particles of lime sludge shall be reduced to a maximum of
1/4-inch in size.
Hydrated lime shall be mixed with water and applied using approved pressure distributing equipment. the
slurry shall consist of a mixture of approximately one ton of lime to each five hundred (500) gallons of
water but shall not contain more than forty percent (40%) lime. Agitation of the slurry mixture shall be
accomplished by using paddles, recirculating pumps, or a combination of these devices. Constant
agitation of the slurry mixture will be required to keep the lime and water in a uniform mixture. The use of
compressed air to aid in the mixing of the slurry will not be permitted. Lime to be applied as a slurry shall
be spread the same day that the slurry is mixed.
Quicklime shall be spread on the subgrade dry, using approved equipment that has demonstrated its
ability to distribute the lime in controlled and uniform amounts. Water shall not be added to the quicklime
until it is thoroughly mixed into the subgrade soil.
Dry lime shall not be applied when the wind conditions are such that blowing lime will be objectionable to
traffic or adjacent property owners.
The quantity of water necessary for the first mixing operation will vary with the nature of the soil and
normally will be three to five percent (3-5%) above the optimum moisture content of the treated soil
mixture. Sufficient water shall be added during the first mixing process to insure proper chemical reaction
between the lime and soil.
402.5 INITIAL CURING
When proper first mixing has been accomplished, the mixture shall be placed in a windrow or spread over
the roadbed and the surface sealed by lightly rolling with a flat steel wheel or pneumatic roller to retard
the loss of moisture and aged for a period of not less than forty-eight (48) hours. The aging process may
be shortened, with the approval of the Engineer, depending upon the type of soil involved. The mixed
material shall be maintained in a moist condition of not less than two percent (2%) below optimum
moisture during the aging process.
402.6 RE-MIXING AND COMPACTION
After the required initial curing time, the soil-lime material shall be re-mixed and pulverized by approved
methods until one hundred percent (100%) of the mixed material by dry weight passes a one and one-half
inch (1 1/2") sieve and at least sixty percent (60%) by dry weight will pass a No. 4 sieve, exclusive of
stone and gravel. The moisture content of the mixed material shall be adjusted during the final mixing
process so that the moisture at the time of compaction will be within two percentage (2%) points above or
below the optimum moisture of the mixed material.
Compaction and finishing operations shall proceed immediately upon completion of the final mixing.
Sheepsfoot rollers shall be used in compaction operations so that the compaction of the mixture will begin
at the bottom and shall continue until the entire depth of mixture is uniformly compacted to the specified
density. The moisture content shall be maintained within two percentage (2%) points of the optimum
moisture during compaction operations. The mixture shall be laid and compacted to a density of at least
ninety-five percent (95%) of the standard density of the soil-lime mixture as determined by the Engineer.
Light sprinkling may be required during laying and compacting operations to maintain the specified
moisture content. Compaction shall be accomplished with sufficient blading to eliminate all irregularities.
The surface shall be lightly scarified during finishing operations and bladed to eliminate any imprints left
by the equipment. Final rolling of the completed surface shall be accomplished with a flat steel roller. The
subgrade shall be brought to a true grade immediately in advance of placing pavement. The surface of
the roadbed shall then be adjusted by cutting off the high areas and filling in the low areas as indicated by
the screed or template. The fill in low areas is to be compacted to the same density requirement as
402.7 FINAL CURING
Upon completion of the compaction and finishing of the treated subgrade no vehicles or equipment other
than sprinkling equipment shall be permitted upon the treated subgrade for a period of seven days;
however, the seven-day curing may be reduced to whatever period of time is required for the treated
subgrade to gain sufficient stability to support the construction equipment if the construction of the
pavement on the treated subgrade takes place in less than the seven-day period after the completion of
the lime treatment. Any damage to treated subgrade due to other phases of construction shall be repaired
at the Contractor's expense. The treated subgrade shall be cured by lightly sprinkling the surface with
water at frequent intervals to prevent drying during the seven-day curing period or until the pavement is
This page was left blank for future use.
PORTLAND CEMENT/FLY ASH TREATED SUBGRADE
This work consists of incorporating Portland Cement or Fly ash, as stabilizing agents, into prepared
Fly ash shall meet requirements of ASTM C-618, Class C, and shall come from a source approved by the
Portland cement shall be Type I/II and shall meet the requirements of ASTM C-150.
403.3 SUBGRADE PREPARATION
Prior to the application of cement or fly ash, the subgrade shall be brought to the proper elevation,
removing all soft spots as described in Section 401.
The surface of the subgrade shall be scarified to a depth necessary to provide the quantity of material,
which when combined with the cement/fly ash, will produce a compacted subgrade of the thickness
designated on the plans. The scarified soil shall be processed with approved graders, discs, harrows, or
rotary mixers until 75 percent (75%) of the soil, by dry weight, exclusive of gravel or stone, shall pass a
No. 4 sieve. The requirement of 75 percent (75%) passing the No. 4 sieve may be waived at the direction
of the Engineer for predominately coarse sandy soils, but the Contractor shall still pulverize the soil to the
extent that homogenous mixture of soil and cement/fly ash can be obtained. The use of gang plows or
blades will be required in this operation to insure that the full depth of material will be loosened from the
subgrade and pulverized. The length of roadway scarified and pulverized at any time shall not exceed the
length which can be completed in accordance with these specifications in two working days, except by
special permission from the Engineer. The soil shall be manipulated and brought to a moisture content of
not greater than three percentage (3%) points below the optimum moisture of the soil involved before
application of the cement/fly ash.
Application rates for cement/fly ash will be determined by the Engineer, consistent with the various types
of subgrade soils. Application shall not be performed when the subgrade is frozen, the temperature in the
shade is less than 50 degrees Fahrenheit for cement or 40 degrees Fahrenheit for fly ash, or when wind
conditions are such that blowing material becomes objectionable to traffic or adjacent property owners.
The soil and cement/fly ash mixture shall extend to a depth of six inches (6") and for a distance of eight
inches (8") beyond the back of the curb lines of the pavement unless indicated otherwise by the plans or
Either bagged or bulk cement may be used. When bulk cement is used, approved spreading and
weighing equipment shall be provided by the Contractor. When bagged cement is used, the
manufacturer's bagged weights shall be accepted to determine the rate of application. Bags shall be
placed in a uniform and regular pattern on the subgrade and the frequency of placing shall be determined
by rate of application. The bags shall then be opened and the cement spread evenly over the subgrade
using a motor grader or other approved method.
Fly ash shall not be applied by the slurry method. The fly ash shall not be placed on wet subgrade or
otherwise allowed to become wet during application.
403.5 MIXING AND COMPACTION - CEMENT
Cement shall be added as previously specified upon completion of the soil preparation. The cement and
soil shall be thoroughly mixed prior to addition of any water. The equipment used in all mixing shall be
such that a uniform mix for the full depth of the material will be assured. Any mixture of soil and cement
that has not been compacted shall not remain undisturbed for more than thirty minutes. Water shall be
added to the soil-cement mixture upon completion of the dry mixing by the use of pressure distributors.
Each application of water shall be partially mixed to avoid a concentration of water near the surface. The
addition of water shall be controlled so that the moisture content of the completed mixture falls inside a
range from optimum to five percent (5%) above optimum moisture of the soil-cement mixture. Sufficient
water distribution equipment shall be used to insure the continuous application of all water required on the
section of roadway being processed within a two-hour period. The mixing of the soil-cement mixture and
water shall be done with discs, harrows, blades, plows, and tillers until the full thickness of the material is
thoroughly and uniformly mixed.
Compaction shall begin within thirty (30) minutes after the material has been mixed and spread. The full
thickness of the material shall be compacted to a density of not less than 95 percent (95%) of standard
compaction of the soil-cement mixture as determined by the Engineer. The compaction operation shall be
sufficient to compact the section of roadway being processed within a period of two (2) hours after
compacting operations begin. Sufficient light blading shall be done during the compaction operations to
blade out all irregularities and to insure a smooth finished surface conforming to the plan cross-section.
Enough sprinkling shall be done during the compaction operation to insure that the moisture content of
the mixture will stay in the required range.
Cement shall be applied only to such an area that all operations from the application of the cement to the
final compaction can be continuous, and all compaction and finishing completed within a period of six (6)
hours after the beginning of the water application to the mixed soil-cement. When any of the operations
after application of the cement are interrupted for a period of more than two (2) hours for any reason, or
when the uncompacted soil cement mixture is wetted by rain so that the average moisture content at the
time of completing compaction is greater than five percentage (5%) points above the optimum moisture
content, the entire section affected shall be reconstructed in accordance with these specifications by the
Contractor at his expense.
The surface of the cement-treated base shall be trimmed to the required line and grade by means of
equipment which is automatically controlled with regard to both longitudinal and transverse slopes.
The Engineer may waive the use of automatically controlled equipment on narrow widths or areas of
irregular dimensions where operation of the automated equipment is impractical.
When required, the surface shall be lightly scarified to loosen any imprints left by the compacting and
shaping equipment. The resulting surface then shall be thoroughly rolled with steel-wheel or pneumatic-
tired rollers or both.
The surface of the material shall be kept moist during all finishing operations. Surface compaction and
finishing of the section being processed shall be done in such a manner as to produce a relatively
smooth, dense surface, essentially free of surface compaction planes, cracks, ridges or loose material.
The completed base course shall conform to the grades, lines and typical cross section shown on the
plans with compacted and dressed edge slopes and all evidence of laps between the various sections
eliminated. With the approval of the Engineer, surface finishing operations may be varied, provided the
quality of the work is as outlined above.
Sufficient equipment shall be in operation on the project so that all operations can be carried on in their
proper sequence without delay and so that final compaction, rolling and finishing can be completed during
At the end of each day's operations, or in case of construction delays that will cause operations to cease,
and at a point where satisfactory construction has been completed, a straight transverse construction joint
shall be formed by cutting back into the completed work to form a true vertical face. A protective covering
of earth shall be placed on the newly constructed base course for a distance back of the joint required for
the turning of equipment used on the following day's work. The thickness of the covering shall be such
that the equipment will not mar or damage completed work.
403.6 MIXING AND COMPACTION - FLY ASH
Mixing of the fly ash with the subgrade soil shall follow application and spreading as a continuous
construction operation. Mixing lifts shall not exceed plan lift thickness unless previously approved. Work
areas for mixing shall not exceed 5,000 square yards unless otherwise authorized by the Engineer.
The mixing procedure shall be as hereinafter described:
a) First Mixing. The moisture content of the subgrade soil shall not exceed eighty percent (80%) of
optimum at the time of first mixing. The soil and fly ash shall be mixed until a uniform mixture is
obtained in which all clods and non-aggregate lumps are reduced to a maximum of two and one-
half inches (2.5") diameter size. The addition of water will not be permitted during first mixing.
First mixing operations shall begin no later than four (4) hours after application of the fly ash.
When deemed necessary by the Engineer, any portion of the work area shall be re-scarified and
additional fly ash added to insure adequate soil modification.
The fly ash and soil shall be thoroughly mixed to the satisfaction of the Engineer prior to the
beginning of final mixing operations.
b) Final Mixing. After the dry soil and fly ash have been satisfactorily mixed, additions of water
shall be made in the final mixing operations to initiate soil-fly ash reaction. The method of mixing
shall be an approved procedure utilizing a traveling rotary mixing plant which demonstrates
uniform dispersion of fly ash and water throughout the soil materials. The quantity of water
necessary for the final mixing operations will vary with the nature of the materials, normally two to
five percentage (2-5%) points above the optimum moisture content of the compacted modified
soil. Sufficient water in any case shall be added in the final mixing process to insure chemical
reaction between the fly ash and soil.
All clods shall be reduced in size by mixing until the soil-fly ash mixture meets the following size
requirements when tested with laboratory sieves:
Sieve Size Percent Passing 1 1/2 inch 100 3/4 inch 50-100
The following alternate mixing procedure may be used at the option of the Contractor and with the
approval of the Engineer in lieu of the procedure described in the above paragraphs. The
moisture content of the soil shall be adjusted to between two (2) and five (5) percentage points
above optimum prior to application of any fly ash. Fly ash shall then be applied and mixing shall
begin immediately. The soil and fly ash shall be mixed until a uniform mixture is obtained in which
all clods and non-aggregate lumps are reduced to a size such that one hundred percent (100%)
will pass a one and one-half inch (1 1/2") screen and fifty percent (50%) to one hundred percent
(100%) will pass a three quarters inch (3/4") screen. Sufficient water shall be added in this mixing
process to insure chemical reaction between the fly ash and water throughout the soil materials.
Compaction shall begin immediately after the mixing is completed when this prescribed
procedure is used.
Compaction of the soil-fly ash mixture shall be performed immediately after final mixing, wherein the
compaction operation shall be a continuation of the final mixing operation. Each lift of mixed fly ash-soil
material shall be compacted full depth to a density of not less than ninety-five percent (95%) of standard
compaction of the fly-ash soil material as determined by the Engineer.
The soil-fly ash mixture shall be compacted without delay and before any appreciable loss of mixing
moisture occurs. Mixing and compaction operations shall be performed in such a manner that the mixture
will be compacted within plus or minus three percentage (3%) points of optimum moisture content.
However, when deemed necessary by the Engineer during the course of construction, changes or
adjustments in the specified moisture requirements to meet field conditions may be authorized.
Compaction shall continue until the entire depth of the mixture is uniformly compacted. The rate of
operation and the number of rollers shall be sufficient to compact uniformly the section of roadway being
processed within two (2) hours after introduction of water.
During the early stages of subgrade construction, the Engineer will work closely with the Contractor by
reporting compaction test results promptly for each stage of fly ash modified subgrade construction as an
aid to the Contractor to establish a construction procedure that will attain the required density within the
prescribed two (2) hours.
The material shall be sprinkled and rolled. All irregularities, depressions or weak spots which develop
shall be corrected immediately by scarifying the areas affected, adding or removing material as required,
and reshaping and recompacting by sprinkling and rolling.
In addition to the requirements specified for density, the full depth of the material shown on the Plans
shall be uniformly compacted to the extent necessary to remain firm and stable under construction
equipment. After each section is completed, density tests as necessary will be made by the Engineer. If
the material fails to meet the density requirements, it shall be reworked as necessary to meet these
requirements. Rework shall include the addition of more fly ash at a rate determined by the Engineer.
Throughout this entire operation the shape of the course shall be maintained and the surface upon
completion shall be smooth and in conformity with the typical sections shown on the Plans and to the
established lines and grades. Should the material, due to any reason or cause, lose the required stability,
density or finish before the next course is placed or the work is accepted it shall be recompacted and
refinished at the sole expense of the Contractor.
403.7 CURING AND PROTECTION
The completed cement/fly ash treated subgrade shall be protected against loss of moisture for a period of
seven (7) days. The curing time may be reduced to a minimum period of three (3) days only when
approved by the Engineer and as further determined by individual project conditions. The completed
cement/fly ash treated subgrade shall be protected against loss of moisture by covering with an approved
moisture barrier such as moist burlap or polyethylene sheet, or at the option of the Contractor and at his
own expense, an application of emulsified asphalt may be applied, using approved pressure-distributing
equipment immediately after the completion of the finishing operations. The asphalt emulsion shall
contain not less than forty percent (40%) of asphalt and shall preferably be of the quick-breaking type of
Immediately prior to the application of the bituminous curing membrane, however, the surface shall be
thoroughly wetted by means of approved pressure-distributing equipment. No free water shall remain on
the surface when the bituminous material is applied. The Contractor shall keep all traffic off the cement/fly
ash-treated subgrade after the curing medium has been applied and until the base has cured for the
specified length of time.
The Contractor shall be required to maintain, at his own expense, the entire roadway within the limits of
the improvement, in good condition, satisfactory to the Engineer, from the time he first starts work until all
work has been completed. Maintenance shall include immediate repair of any defects that may occur
either before or after the cement/fly ash is applied to the subgrade soil.
Cement/fly ash treated subgrades shall be constructed to elevations such that it will not be necessary to
cut or trim in excess of one inch (1") of material off the subgrade.
This page was left blank for future use.
GEOGRID REINFORCED AGGREGATE BASE
404.1 CRUSHED ROCK BASE FOR CONCRETE PAVER SURFACE
Where the plans and typical sections call for crushed rock base under concrete paver surfaces, the
materials used shall be crushed concrete meeting the specifications for size and gradation for crushed
rock base. Any additional costs for crushed concrete or for extra thickness as shown on the details will be
incidental to the bid item.
Materials to be used for geogrid reinforced base construction shall consist of virgin crushed stone,
recycled Portland cement concrete, or Reclaimed Asphalt Pavement (RAP).
Sieve Size Percent % Retained
(by dry weight) 2-1/2" 0 3/4" 20-60 #4 50-80 #40 80-94 #200 90-98
Base material quality shall conform to the requirements specified by the KDOT Subsection 1102
for Durability Class 1.
All virgin base material shall have a maximum absorption of four percent (4%).
Recycled Asphalt Pavement (RAP)
Recycled Asphalt Pavement (RAP) shall be free of detrimental quantities of organic, non-granular soils
and deleterious materials.
The RAP sub-base shall be a six-inch minimum deep lift of 100 percent pulverized asphalt concrete
compacted to at least ninety-five percent (95%) of Standard Proctor with a moisture content equal to or
greater than optimum. A moisture-density relationship may be prepared in advance with RAP that will be
delivered to the project.
The maximum size of the RAP particles shall be 1-1/2 times the maximum aggregate size in the RAP
RAP sub-base shall be compacted and smoothed with a steel-faced roller prior to placement of asphalt.
Tack coat will not be applied to RAP.
The geogrid shall be a regular grid structure formed by biaxially drawing a continuous sheet of select
polypropylene material and shall have aperture geometry and rib and junction cross-sections sufficient to
permit significant mechanical interlock with the material being reinforced. The geogrid shall maintain its
reinforcement and interlock capabilities under repeated dynamic loads while in service and shall also be
resistant to ultraviolet degradation, to damage under normal construction practices and to all forms of
biological or chemical degradation normally encountered in the material being reinforced.
The geogrid shall be BX100 by Tensar Corporation, or approved equal, and shall also conform to the
PROPERTY TEST METHOD UNITS VALUE
= aperture size1 I.D. Calipered
= MD in 1.0 (nom)
= CMD in 1.3 (nom)
= open area CDE Method3 % 70 (min)
= thickness ASTM D 1777-64
= ribs in 0.03 (nom)
= junctions in 0.11 (nom)
= flexural rigidity ASTM D1388-644 mg-cm 250,000 (min)
- modulus GRI GG1-875 lb/ft 13,500 (min)
- @ 2% strain GRI GG1-875 lb/ft 270 (min)
- @ 5% strain GRI GG1-875 lb/ft 540 (min)
- ultimate strength GRI GG1-875 lb/ft 850 (min)
= junctions GRI GG2-876
= strength lb/ft 750 (min)
= efficiency % 90 (min)
= polypropylene ASTM D 4101 % 98 (min)
Group 1/Class 1/Grade 2
= carbon black ASTM 4218 % 0.5 (min)
Minimum Dimensions & Weights
= roll length ft 164
= roll width ft 9.8 & 13.1
= roll weight lb 71 & 95
Notes: 1. MD dimension is along roll length. CMD dimension is across roll width. 2. Maximum inside dimension in each principal direction measured by calipers. 3. Percent open area measured without magnification by Corps of Engineers method as specified in CW 02215 Civil Works Construction Guide, November 1977. 4. ASTM D 1388-64 modified to account for wide specimen testing as described in Tensar test method TTM-5.0 "Stiffness of Geosynthetics". 5. Secant modulus at 2% elongation measured by Geosynthetic Research Institute test method GG1-87 "Geogrid Tensile Strength". No offset allowances are made in calculating secant modulus. 6. Geogrid junction strength and junction efficiency measured by Geosynthetic Research Institute test method GG2-87 "Geogrid Junction Strength".
404.3 CONSTRUCTION REQUIREMENTS
Prior to placement of the geogrids, the subgrade shall be prepared as described in Section 401.
Placing and Overlapping Geogrids
Place geogrids in position and roll out over the prepared subgrade. Geogrid should be cut to conform to
manhole covers or other protrusions. Geogrid should be cut and overlapped as necessary to
accommodate curves. Pin overlaps to secure against separation and to provide anchorage. If two rolls
are to be placed side by side, or end to end, overlap them as noted in Table 1.
Table I: Recommended Overlaps
Soil Type CBR Grid Overlap
Firm > 2 1'
Soft Ground 1-2 2'
Very Soft Ground < 1 3'
Overlap geogrids in the direction fill will be spread. Over very soft ground, wire, plastic ties or hog rings
can be used on five to twenty-foot spacings as necessary to secure the overlaps.
Tensioning and Pinning
Pin beginning of roll to the ground with six-inch (6") "U" staples or other approved fastener. Pin at edges,
overlaps, and center of roll width. Over soft ground it may only be necessary to secure the end with
stakes, rocks, or fill.
Pull geogrids tight by hand to take up all slack.
a) Firm Ground. Anchor geogrid to the ground at edges, including overlaps, and in center of roll on
thirty foot (30') intervals along the roll length.
b) Soft Ground. Anchor only the roll ends. The geogrids will conform to the ground surface as the
fill material is dumped.
Anchor the terminal ends of the roll. If the overlap is required for advancing rolls, overlap as noted
previously and anchor at the overlap.
Dumping and Spreading
a) Soft Subgrade. Back Dump or End Dump and Spread. Thin fill lifts over very soft subgrades may
not be sufficient to support loads of fill and heavy equipment. Low ground pressure tractors and
low tire pressures (less than 4 psi) are recommended for hauling and spreading fill over these
conditions. Do not operate equipment directly on the grid. Insure at least four inches (4") of fill is
between the grid and vehicle.
Back dump specified fill onto the geogrid where subgrade is most stable. Spread the fill material
over the geogrid out toward the softer subgrade.
Grade fill to the specified thickness. Raise the blade gradually as the fill is pushed out over the
grid. This causes much of the fill to roll out onto the grid and reduce stresses on the subgrade.
Back dump subsequent loads onto the leveled fill and advance forward by spreading with a
b) Firm Subgrade. Dump while driving over. Adequate anchoring is required in this case to prevent
haul traffic from pushing or shifting grid out of position on the ground.
Rubber tire trucks (end and belly dumps) can drive over the grid at very slow speeds, less than 5
mph, and dump fill as they do. Avoid turning and sudden stops. Do not drive tracked vehicles
directly on the grid. Ensure at least four inches (4") of fill is between the grid and tracks.
Back Dumping can be employed over firm ground as described for soft ground conditions.
Grade fill material to desired thickness. Raise the blade while leveling fill.
Crown fill during the grading process to assure rainfall runoff and prevent fill saturation.
Compact fill to project specifications after it is graded smooth and before it is open to truck traffic.
Inadequate compaction will result in surface rutting under wheel loads. This reduces the total thickness of
the fill and increases stress on the subgrade. Note: Compaction equipment should be appropriate for the
type of fill used and subgrade conditions that exist. Do not use vibratory compactor on fill over very soft
saturated subgrades. It may cause a "quick" condition resulting in rapid subgrade strength loss.
Should the geogrid be damaged during or after installation, repair by patching.
Remove fill from the surface of the grid at the damaged area and three feet (3') around in all directions.
Place a geogrid patch of appropriate dimensions to cover damaged area and extending three feet beyond
in all directions.
Replace fill and compact.
Rock base is to be compacted and smoothed with a steel faced roller prior to placement of asphalt or
concrete pavement. Tack coat will not be applied to rock base.
ASPHALTIC CONCRETE PAVEMENT
This item shall consist of leveling, surface and/or base courses and curbs placed upon the previously
prepared base or subgrade in accordance with these specifications to the compacted thickness and
design shown on the plans or ordered in writing by the Engineer.
405.2 MATERIALS AND MANUFACTURE:
The approval of sources of supply for stone, gravel, sand, and mineral filler supplement to be used in
asphaltic mixtures shall be obtained from the Engineer prior to delivery to the project and samples of each
aggregate or mineral filler shall be submitted for testing as directed by the Engineer. All test procedures
shall be conducted in accordance with the latest standards or tentative standards of the American Society
for Testing and Materials. Individual aggregates having more than ten percent (10%) retained on the No.
8 sieve shall have a percent of wear of not more than forty percent (40%) when tested by the Los Angeles
Abrasion Test Method. Individual aggregates having more than ten percent (10%) retained on the No. 8
sieve shall have a loss of not more than fifteen percent (15%) when tested by the Sodium Sulfate Method
as specified in the latest revision of ASTM C-88. That portion of individual aggregates retained on No. 30
sieve shall have a maximum absorption of four percent (4%). Individual aggregates used in surface
course mixes which have more than ten percent (10%) retained on the No. 8 sieve shall have a loss of
not more than eighteen percent (18%) when tested by the Magnesium Sulfate Method as specified in
All aggregates and mineral filler supplements to be used in asphaltic mixtures shall be free from alkali,
acids, organic matter, or injurious quantities of other foreign substances. Other deleterious substances in
each individual aggregate or mineral filler supplement shall not exceed the following percentages by
Substance Max. %
Sticks (wet) 0.1%
Shale, shale like, or soft friable material, singly or in combination 3.0%
a) Crushed Rock
Crushed rock shall be produced from durable rock. The crushed rock shall have a percent of
wear of not more than forty percent (40%) when tested by the Los Angeles Abrasion Test
Method. Crushed rock shall be of uniform quality throughout, without an excess of flat or
elongated pieces and it shall be clean and free from dust such that not more than four percent
(4%) of the material will pass the No. 200 sieve.
b) Crushed Gravel
Crushed gravel shall be produced by crushing siliceous or calcareous gravel. At least ninety
percent (90%) of the particles retained on the No. 4 sieve shall have one or more fractured faces
to be considered as crushed gravel. The screenings resulting from the crushing of gravel will not
be considered as crushed aggregate. Crushed gravel shall be clean and free from dust such that
not more than four percent (4%) of the material will pass the No. 200 sieve. Crushed gravel
having more than ten percent (10%) retained on the No. 8 sieve shall have a percent of wear of
not more than forty (40%) when tested by the Los Angeles Abrasion Test Method.
Sand-gravel shall be a mixture of natural sand and gravel formed by the disintegration of siliceous
and/or calcareous rocks. Natural sand shall consist of particles of aggregate resulting from the
natural disintegration of siliceous and/or calcareous rocks. Manufactured sand shall be produced
by crushing predominately siliceous sand and gravel. Sand-gravel having more than ten percent
(10%) retained on the No. 8 sieve shall have a percent of wear of not more than forty (40%) when
tested by the Los Angeles Abrasion Test Method. That portion of sand-gravel passing the No. 40
sieve shall have a plasticity index of not more than 6. Sand-gravel shall be graded such that not
more than twenty percent (20%) will pass a No. 200 sieve.
Chat shall consist of mine run or screened tailings produced during the milling of lead and zinc
ores in the mining district of Southeast Kansas, Southwest Missouri, and Northeast Oklahoma.
Chat shall be graded such that when mixed with the other aggregates the combined gradation will
conform to the specified requirements.
Screenings shall be produced by crushing aggregates that meet the quality requirements for
crushed rock. The gradation shall be such that not more than two percent (2%) will be retained on
the three eighths inch (3/8") sieve and not more than forty percent (40%) will pass the No. 200
sieve. That portion of screenings passing the No. 40 sieve shall have a plasticity index of not
greater than 6.
f) Mineral Filler
Mineral filler is defined as that portion in the final combined mix that is finer than the No. 200
sieve. Material to supplement the mineral filler in the coarser aggregates, when required, shall
consist of Portland cement, pulverized limestone, hydrated lime, or processed and dewatered
chat sludge. All mineral filler supplements shall meet with the approval of the Engineer. Mineral
filler supplements shall be free from cemented lumps and must be easily pulverized. The blending
of two or more materials to produce a mineral filler supplement will not be permitted. Material to
be used as a mineral filler supplement shall have a plasticity index of not greater than 6. Hydrated
lime or Portland cement to be used as a mineral filler supplement shall conform to the same
requirements as specified for these materials in the specifications for treated subgrade, Sections
402 and 403. Pulverized limestone and processed chat sludge shall be graded such that not
more than forty percent (40%) of the material will be retained on the No. 200 sieve when used as
a mineral filler supplement. Silt will have a minimum of fifty percent (50%) passing the 200 sieve.
Asphalt cement shall be of uniform consistency, free from water to the extent that it will not foam when
heated to three hundred fifty degrees (350) F., and it shall meet the following requirements for physical
and chemical properties:
Penetration Graded Asphalt Cement
1. Flash point (COC) F.450+
2. Penetration, 77 F., 100g., 5 secs. 60 to 70
3. Ductility at 77 F., 5 cm./min., cm 100+
4. Loss at 325 F., 5 hours, percent 1.0-
5. Penetration of residue at 77 F., 100g., 5 secs.,
as compared to penetration before heating, percent 75+
6. Solubility, percent 99+
Viscosity Graded Asphalt Cement
Viscosity, 140 F., poises 1600 min. - 2400 max.
Viscosity, 275 F., centistokes 300 min.
Penetration, 77F., 100 g., 5 sec. 60 min.
Flash Point (COC), F 460 min.
Solubility, percent 99.0 min.
Loss on heating, thin-film oven test 0.5% max.
Tests on Residue from Thin-Film Oven Test
Viscosity, 140 F., poises 8000 max.
Ductility, 77 F., 5 cm. min., cm 50 min.
Penetration graded asphalt cement may be changed during cold weather construction on residential
streets from a 60-70 penetration at seventy-seven degrees (77) F., 100 grams, 5 seconds to an 85-100
penetration at seventy-seven degrees (77) F., 100 grams, 5 seconds when requested by the Contractor
and approved by the Engineer. Viscosity graded asphalt cement may be changed during cold weather
construction on residential streets from a viscosity of 2000 400 poises at 140F. to a viscosity of 1000
200 poises at 140F. when requested by the Contractor and approved by the Engineer. No additional
compensation will be made for this change in grade of asphalt cement. Viscosity graded asphalt cements
shall not be mixed with penetration graded asphalt cements.
All asphalt cement used on any one project shall be penetration graded or viscosity graded at the
Contractor's option. The Contractor will be permitted to change asphalt grades on any one project only in
the event of unavailability of asphalt from his initial source and with the provision that his storage tanks
are drained prior to changing from one type of grading to the other type of grading. Asphalt mixes shall be
redesigned whenever a change in asphalt grading is permitted.
Polymer Modified Asphalt Cement
The material shall consist of an asphalt cement to which a styrenebutadiene polymer has been added.
The polymer modified asphalt cement shall be smooth, homogeneous and comply with the following
________________________________________ 1 Solubility of original asphalt by ASTM D2042
a) Property Type 1C Type 1D
Penetration @ 77F, 100g, 5 sec.: Min 50 40
Max 75 75
Penetration @ 39.2F, 200g, 60 sec.: Min 25 25
Viscosity, @ 140F1, Poise: Min 5000 5000
Viscosity, @ 275F, cSt: Max 2000 2000
Ring & Ball Softening Point, F: Min 130 140
Flash Point, F: Min 450 450
Solubility in Trichloroethylene, % Min 99.0 99.0
Separation,3 Ring & Ball difference, F: 4 4
b) Test for Elasticity (after aging)
Elastic Recovery4, 77F, % Min45 50
c) Tests on Residue from Rolling Thin-film Oven Test
Penetration @ 39.2F, 200g, 60 sec.: Min13 13
2 Stiffer mix generally used in intersections to prevent rutting. 3 Procedure attached 4 Procedure attached
The separation of polymer from asphalt during hot storage is evaluated by comparing the ring and
ball softening point of the top and bottom samples taken from a conditioned sealed tube of
polymer modified asphalt. The conditioning consists of placing a sealed tube of polymer modified
asphalt in a vertical position in a 325F oven for a 48-hour period.
ASTM D36: Softening Point of Bitumen (Ring and Ball Apparatus)
ASTM E11: Specifications for Wire Cloth Sieves for Testing Purposes
Aluminum Tubes1 - 1 inch diameter by 5-1/2 inch length blind aluminum tubes. Used to hold the
test sample during the conditioning.
Oven - An oven capable of maintaining 325 + 10F
Freezer - A freezer capable of maintaining 20 + 10F
Rack - A rack capable of supporting the aluminum tubes in a vertical position in the oven and
Spatula and Hammer - The spatula must be rigid and sharp to allow cutting of the tube
containing the sample when at a low temperature.
Place the empty tube with sealed end down in the rack. Carefully heat the sample until sufficiently
fluid to pour. Care should be taken to avoid localized overheating. Strain the melted sample
through a No. 50 sieve conforming to ASTM E11. After thorough stirring, pour 50.0 grams into the
vertically held tube. Fold the excess tube over two times and crimp and seal.
Place the rack containing the sealed tubes in a 325 + 10F oven. Allow the tubes to stand
undisturbed in the oven for a period of 48 + one hour. At the end of the heating period, remove
the rack from the oven and immediately place in the freezer at 20 + 10F taking care to keep the
tubes in a vertical position at all times. Leave the tubes in the freezer for a minimum of four hours
to completely solidify the sample.
Upon removing the tube from the freezer, place the tube on a flat surface. With the spatula and
hammer, cut the tube into three equal length portions. Place the beakers in a 325 + 10F oven
until sufficiently fluid to remove the pieces of aluminum tube.
After a thorough stirring, pour the top and bottom samples into appropriately marked rings for the
ring and ball softening point test. Prepare the rings and apparatus as described in ASTM D36.
The top and bottom sample from the same tube should be tested at the same time in the
softening point test.
________________________________________ Aluminum tubes may be obtained from Sheffield Industries, P.O. Box 351, New London, CT 06320,
203/442-4451. Observations have been reported regarding leakage of asphalt from the bottom of these
tubes during the conditioning period.
d) Separation Test for Type I Polymer Modified Asphalt:
1 Other tubes may be required if this leakage is significant
2 Other physical and chemical residue tests may be run at this time, if desired.
Record the softening point of the top and bottom portions of the sample. Duplicate separation
tests should be run. d. Elastic Recovery Test
The elastic recovery of a polymer modified asphalt cement is evaluated by the percentage of
recoverable strain measured after elongation during a conventional ductility test. Unless
otherwise specified, the test shall be made at a temperature of 77F + 0.9F (25 + 0.5C) and
with a speed of 5 cm/min + 5.0%.
ASTM D113: Ductility of Bituminous Materials
ASTM E11: Specifications for Wire Cloth Sieves for Testing Purposes
Mold - The mold shall be similar in design to that described for use in the ductility test (ASTM
D113), Figure 1, except that the sides of the mold assembly, parts a and a' shall have straight
sides producing a test specimen with cross-sectional area of 1 cm
Water Bath - The water bath shall be maintained at the specified test temperature, varying not
more than 0.18F (0.1C) from this temperature. The volume of water shall be not less than 10
cm and shall be supported on a perforated shelf not less than 5 cm from the bottom of the bath.
Testing Machine - For pulling the briquet of bituminous material apart, any apparatus may be
used which is so constructed that the specimen will be continuously immersed in water as
specified while the two clips are pulled apart at a uniform speed without undue vibration.
Thermometer - An ASTM 63C or 63F thermometer shall be used.
Scissors - Any type of conventional scissors capable cutting polymer modified asphalt at the test
Procedure: Prepare test specimens and condition as prescribed by ASTM D113.
Elongate the test specimen at the specified rate to a deformation of 10 cm.
Immediately cut the test specimen into two halves at the midpoint using the scissors. Keep the
test specimen in the water bath in an undisturbed condition for one hour. After the one hour time
period, move the elongated half of the test specimen back into position near the fixed half of the
test specimen so the two pieces of polymer modified asphalt just touch. Record the length of the
test specimen as X.
Report: Calculate the percent recovery by the following procedure:
Recovery, % = 10 - X x 100
Composition of Asphaltic Mixtures
Aggregates, mineral filler and asphalt shall comply with the requirements, as stated previously in
this subsection. The Contractor shall submit to the Engineer before December 31 of each
calendar year a complete listing of Individual Aggregate Sieve Analysis, Mix Combination Sieve
Analysis and any other pertinent data on the mixes to be used during the following calendar year.
The Engineer may use the submitted design in whole or in part, at his discretion. The mix design
shall be adjusted as necessary when a change in the source of materials is approved. Any mix
design that proves to be unsatisfactory shall be adjusted by the Engineer. There shall not be less
than three percent (3%) or more than twenty-five (25%) of material between any two successive
sieves in the following series: No. 4, 8, 16, 30 and 50. The requirements for percent retained on
the No. 200 sieve (dry screen) will be waived, provided the plasticity index of the mineral filler is
four (4) or less.
Salvaged hot mix asphaltic materials may be recycled and combined with new materials to
produce asphaltic base course and surface mixtures for use in construction of such base courses
and surface courses as required by plans. The combination of salvaged hot mix asphaltic material
with new materials shall not exceed twenty-five percent (25%) for base course mixtures or fifteen
percent (15%) for surface course mixtures. All base course mixtures containing recycled asphaltic
material shall conform to the standard specification requirements for a BC-1 type mix, unless
otherwise noted on the plans. All surface course mixtures containing recycled asphaltic material
shall conform to the standard specification requirements for an SC-1 type mix, unless otherwise
noted on the plans.
Mineral Aggregates Percentage by Weight Retained
3/4" 0-12 0 0
1/2" 0-8 0-10
3/8" 2-35 0-18 12-26
#4 18-39 39-56
#8 30-66 35-53 60-76
#16 56-68 72-87
#30 60-82 60-80 79-92
#50 70-88 84-95
#100 80-93 88-98
#200 89-96 90-95 92-98
P-200 4-11 5-10 2-8
The combined material for asphalt surface course, SC-I, shall contain not less than 47 percent crushed
material, including the material passing the No. 200 sieve.
The combined material for asphalt surface course, BM-IB, shall contain not less than 75 percent crushed
material, including the material passing the No. 200 sieve. In addition, course aggregate (#4+) used in
BM-IB shall have a maximum absorption of two percent.
All asphalt mixtures shall conform to the following Marshall requirements when tested in
accordance with the latest revision of ASTM D-1559.
Mix Type BC-I SC-I BM-IB
Min stability 1000 1600 1800
Voids (%) 3-7 3-5 3-5
VFA (%) 70 min. 70 min. 68-78
BM-IB requirements shall be for a 75-blow Marshall.
405.3 PAVING PLANT
All plants used by the Contractor for the preparation of asphalt paving mixtures shall conform to the
applicable sections of the KDOT Standard Specifications unless specified otherwise. All bins used in
storing mixed asphalt material shall be completely enclosed. All elevators used to handle mixed asphalt
materials during periods of adverse weather conditions shall be completely enclosed. Adverse weather
conditions shall be defined either as rainy or foggy weather, prevailing temperatures of less than sixty
degrees (60) F., or gusting and prevailing winds over twenty (20) miles per hour.
The Contractor shall have the option, with the approval of the Engineer, to operate the asphalt plant
without screening the coarse and fine aggregates into separate bins. The basic concepts of this method
of operation are to remove all plant screens, with the exception of the scalping screen, and to test and
accept each individual aggregate prior to entering the drier. Permission to continue under this option may
be rescinded upon failure to maintain acceptable production. All methods of plant operation without
screens shall conform to applicable sections of the latest edition of the KDOT Standard Specifications,
except that the material produced will meet the requirements as set out in these Specifications.
Asphalt paving mixtures may be prepared by using a drum mix type asphalt plant when approved by the
Engineer. The approval of and continued use of a drum mix type asphalt plant shall be contingent upon
its ability to proportion and mix satisfactorily the required materials in accordance with the specifications
such that the finished work will be equal to the work produced as if accepted standard methods had been
405.4 PAVING PLANT OPERATION
Sand and Stone Storage. The different kinds of sand and stone used shall be kept separate, using such
provisions as deemed necessary by the engineer to keep them from becoming mixed.
All aggregates for surface mixture shall be delivered to a revolving drier. The aggregates shall be heated
to a temperature of between 275 degrees F. and 350 degrees F. The aggregate shall then be weighed in
accordance with the approved mix. Each batch shall be mixed by first charging the mixer with the coarse
and fine aggregate along with the mineral filler and thoroughly mixed, then the asphalt cement shall be
added and the mixing continued for at least 45 seconds or longer if necessary to produce a homogenous
mixture in which all particles of the aggregate are uniformly coated.
The asphalt cement shall be delivered to the surface mixture at a temperature of 275 degrees F. to 350
The paving plant operation shall conform to the requirements of applicable sections of the latest edition of
the KDOT Standard Specifications when plant operations without screening the coarse and fine
aggregates into separate bins is permitted.
When the Engineer has approved the use of a drum mix type asphalt plant the sections in these
specifications which do not conform to this method shall not be applicable. Approval of and continued use
of a drum type asphalt plant shall be contingent upon the results obtained in the completed work.
The Contractor shall give to the Engineer notice of intent to mix and place asphalt materials as far in
advance as is possible and the minimum time for such notification shall be four hours. Asphalt materials
shall be mixed only when the City's inspector is at the plant site, unless approved otherwise by the
Engineer. Mixed asphalt material that has been stored over night shall not be used unless written
permission is given by the Engineer.
405.5 CONSTRUCTION REQUIREMENTS
Equipment used in the construction of asphalt pavements such as hauling equipment, bituminous pavers,
heating equipment, bitumen distributors, compacting equipment, and weighing equipment shall conform
to the applicable sections of the latest edition of the KDOT Standard Specifications.
405.6 PREPARATION OF THE BASE
Prepared Subgrade or Geogrid Aggregate Base
After the road bed has been prepared, as described in Sections 401-404, it shall be maintained during
asphalt placement until completely covered. It shall be the Contractor's sole responsibility to maintain the
subgrade as prepared, and any defect which may develop shall be corrected at his expense.
Existing Bituminous Surface
When the surface is constructed on an existing bituminous surface, the surface shall be cleaned of all
foreign material and broomed free of dust. In addition, any loose, broken or shattered bituminous material
along the edges of the existing surface shall be removed and the exposed subgrade and a sufficient width
of the shoulder adjacent to the edge of the existing surface to receive the new bituminous mixture shall be
shaped, bladed and broomed to provide a uniform trim subgrade for the new surface course.
The existing mat, base, or subgrade shall be removed through broken, shattered, or unstable areas as
shown on the Plans or designated by the Engineer. The areas shall be excavated to a depth directed by
the Engineer, and refilled with bituminous base mixture.
Concrete or Brick Pavement
If the existing surface is concrete pavement or brick pavement, the pavement shall be cleaned of dirt,
bituminous material and other foreign material, as directed by the Engineer. Bituminous material such as
crack filler or joint material in expansion joints or cracks shall be removed to a depth of at least two inches
(2") when specified by the Engineer. The joints and cracks shall then be refilled with surface course
material and compacted. Wide longitudinal or diagonal cracks caused by the transverse movement of
portions of the pavement shall be cleaned for their full depth and back filled with surface course material
and the material compacted is not to exceed three-inch (3") layers by means of mechanical or hand
tampers equipped with special tamping heads. Crack cleaning and filling shall be done as far in advance
of the leveling course as is practicable.
Prior to the placing of the mixture, when designated by the Engineer, a tack coat shall be applied to the
existing surface. The type of asphalt used shall be emulsified asphalt (CSS-1h), or (SS-1h), and the rate
of application shall be designated by the Engineer, except as set forth below.
Tack coat shall be diluted in the proportion of 50 percent water and 50 percent emulsion and applied at
the rate of 0.05 to 0.10 gallons per square yard. Application shall be made in advance of subsequent
construction as ordered by the Engineer.
Tack coat shall be applied by distributor trucks designed, equipped, and maintained to provide uniform
coverage at the designated application rate. Hand spray by means of hose or bar through a gear pump or
air tank shall be acceptable for resurface work, corners or tacking or vertical edges. Care shall be taken
to provide uniform coverage. Equipment that performs unsatisfactorily shall be removed from the job.
405.7 PLACING REQUIREMENTS
The bituminous mixture shall be spread and finished reasonably true to crown and grade by the
automatically controlled bituminous paver. Bituminous mixtures may be spread and finished by hand
methods only where machine methods are impractical as determined by the Engineer.
The automatically controlled paver shall spread the bituminous mixtures without tearing the surface and
shall strike a finish that is smooth, true to cross section, uniform in density and texture and free from
hollows, transverse corrugations and other irregularities.
The paver shall be operated at a speed which will give the best results for the type of paver being used
and which coordinates satisfactorily with the rate of delivery of the mixture to the paver so as to provide a
uniform rate of placement without undue intermittent operation of the paver.
All mixed material shall be delivered to the paver in time to permit completion of spreading, finishing and
compaction of the mixture during daylight hours. Night time work on projects not open to traffic may be
permitted when ample lighting and other satisfactory measures are provided.
The longitudinal joints in successive courses shall be offset not less than twelve inches (12"). The width of
the surface of the top course placements shall conform to traffic lane edges when possible.
Bituminous mixtures, except on leveling courses, shall be spread in a placement thickness so that after
rolling the nominal thickness of the compacted mat will not in general exceed the following, unless
otherwise specified by the Engineer:
Surface Course Intermediate On fresh subgrade
2" 4" 4"
The maximum thickness for lifts may be increased when such increase is more adaptable to total
pavement thickness and when in the opinion of the Engineer, it is not detrimental to placement and rolling
conditions. The Engineer may adjust lift thickness in order to obtain the most efficient combination of
aggregate type, laydown equipment, mixture characteristics, temperatures and rolling equipment to
produce the required density and surface characteristics.
The Engineer will make the survey required for the reference grade. The Contractor shall erect and
maintain a reference string line and operate the paver to conform to the string line for the initial lift and/or
any lifts if specified by the Engineer.
If automatic profile road building type equipment is used to prepare the subgrade, the requirements for an
erected reference string line may be waived.
The Contractor shall furnish and maintain an approved mobile string line for all lifts not laid with the
erected string line, and operate the paver to conform to that string line. The erected string line shall be
erected parallel to the reference grade, and the bituminous mixture shall be spread at a constant
elevation above, below or at the string line elevation as directed.
The use of the automatically controlled bituminous paver to provide both longitudinal and transverse
control shall include the furnishing and maintaining of a string line, whether it be erected or mobile, by the
Contractor. The longitudinal and transverse controls shall operate independent of each other to the extent
that the surface of the bituminous mixture will reasonably conform to the string line and will be reasonably
uniform in cross-section or crown.
On the initial traffic lane paving operation, the asphaltic mixture shall be spread with the bituminous paver
to grade line constant to the Reference String Line as required.
The erection and maintenance of the Reference String Line shall be so coordinated that the string will be
taut and free from sags at the time it is in use as a guide for the paver.
On second and subsequent lay-downs, the asphaltic mixture shall be spread as described for the initial
lay-down except that the spreading of the asphalt shall conform to the motion of the Mobile String Line.
The Mobile String Line or equivalent shall be used as the reference guide on all paving operations except
when the Reference String Line is used or other provisions are made and approved by the Engineer.
On the new construction where paving starts on fresh earth subgrade, the survey may be delayed to the
surface of the first course and the use of the Reference Grade Line may be delayed to the first lay-down
operation of the second course.
If the existing surface is of acceptable centerline grade as determined by the Engineer from the profile
survey, the Engineer may permit the use of the mobile string line for all lifts.
If the automatic longitudinal and transverse controls breakdown, the Engineer may permit the paver to
operate during the next three (3) calendar days without the automatic controls to allow time for repair, but
it shall not operate on a lift that was laid without automatic controls or if the Plans require only one (1) or
two (2) lifts. The initial lift shall not be laid without automatic controls.
The use of the automatically controlled paver may be waived on irregular sections or other sections as
Spreading and Surface Tolerances
The Engineer shall make checks and adjustments as indicated to maintain the rate of spreading within
the required calculated weight per unit of area so as to produce a compacted lift thickness in substantial
conformity to the design or specified thickness.
Where leveling courses or variable depth courses are specified, the rate of spreading shall be at rates in
accordance with the intent of the Plans or as directed by the Engineer.
The surface will be tested by the Engineer using a ten-foot (10') straight edge at selected locations at the
Engineer's discretion. The variation of the surface from the testing edge of the straight edge between any
two (2) contacts with the surface shall not exceed one-fourth inch (1/4"). All necessary corrections will be
at the expense of the Contractor.
All asphaltic surface course mixtures shall be delivered to the place of construction within a temperature
range of between two hundred sixty degrees (260) F. and three hundred thirty-five degrees (335)F.
Asphaltic base mixtures shall be delivered to the place of construction within a temperature range of
between two hundred twenty degrees (220) F. and three hundred thirty-five (335) F. The temperature of
the asphaltic mixtures shall be regulated within these limits in accordance with the workability of the mix
and the weather conditions. The temperature of the asphaltic materials shall be maintained at the above
indicated maximum temperature when hand spreading and raking of the material is required.
Weather Limitations for Placing Asphaltic Mixtures
Asphaltic mixtures shall not be placed on any wet or frozen surface or when the weather conditions
otherwise are detrimental to the proper handling or finishing of such mixtures. Asphaltic mixtures shall not
be placed when the air temperature as measured in the shade is less than 40F. Asphaltic base course
material with thicknesses of three inches (3") or more may be placed when the air temperature as
measured in the shade is 30F. or above with the approval of the Engineer if density and Marshall
requirements can be obtained.
405.8 COMPACTION OF MIXTURES
After spreading and strike-off and as soon as the temperature and mix conditions permit the compacting
to be performed without excess shoving or tearing, the mixture shall be thoroughly and uniformly
Rollers shall be self-propelled and shall be in good condition, capable of reversing without backlash, and
shall be operated at speeds slow enough to avoid displacement of the bituminous mixture. The number
and weight of rollers shall be sufficient to compact the mixture to the required density while it is still in a
workable condition. The use of equipment which results in excessive crushing of the aggregate will not be
permitted. A minimum of two (2) rollers, one (1) steel wheel and one (1) pneumatic tire type, shall be used
with each spreading operation unless otherwise specified by the Engineer.
Other approved compaction devices may be used in lieu of conventional rollers when approved by the
The selection of the type of roller to be used on the breakdown rolling may be varied to suit mix
characteristics. The final rolling of the top or surface course shall be accomplished with a steel roller
unless otherwise designated. When the specified density is not obtained, changes in size and/or number
of rollers or compactive device shall be made as corrective measures to satisfy the density requirement.
Rollers or other compactive devices shall be operated by competent and experienced roller men and shall
be kept in operation continuously if necessary so that all parts of the pavement will receive substantially
equal compaction at the time desired. The Engineer shall order the mixing plant to cease operations at
any time proper compacting is not being performed.
Any mixture that becomes loose, broken, mixed with foreign material, or which is in any way defective in
finish or density, or which does not comply in all other respects with the requirements of the
Specifications shall be removed, replaced with suitable material, and finished in accordance with these
For specified lift thickness of one and one-half inches (1 1/2") or greater, the bituminous mixture shall be
compacted to a Road Density equal to or greater than the percent of the Field Mold Density as set forth
Type Aggregate Required Field
Bit. Base Course 95%
Bit. Surface Course 95%
Bit. Shoulders (All Agg. Types) 90%
When the lift thickness as specified is less than one and one-half inches (1 1/2"), the bituminous mixture
shall be compacted using a minimum of two (2) approved rollers and in such a manner so as to obtain the
best possible consolidation. If available, non-destructive test methods may be used to establish a suitable
When the area to be compacted is not intended to carry traffic, such as certain types of median areas,
compaction shall be achieved by the best suitable equipment, and density requirements may be waived
by the Engineer.
Contact surfaces of curbing, gutters, manholes and similar structures shall be painted with a thin uniform
coating of emulsified asphalt (CSS-1h) or (SS-1h) material. The bituminous mixture shall be placed
uniformly high near the contact surfaces so that after compaction it will be one-fourth inch (1/4") above
the edge of such structures.
Joints between old and new pavements or between successive day's work shall be made so as to insure
through and continuous bond between the old and new mixtures. Transverse construction joints in
previously laid material may be constructed by cutting the material back for its full depth so as to expose
a fresh surface. Where a wooden header is used at a construction joint, the cutting may be omitted
provided the joint conforms to the specified thickness and cross-section.
Before placing the fresh mixture against a cut joint or against old pavement, the contact surface shall be
sprayed or painted with a thin uniform coat of emulsified asphalt material. Where a finishing machine is
used, the longitudinal joint shall be made by overlapping the screed on the previously laid material for a
width of at least one inch (1") and depositing a sufficient amount of mixture so that the joint formed will be
smooth and tight.
PORTLAND CEMENT CONCRETE PAVEMENT
This item shall consist of a pavement composed of plain or reinforced jointed Portland cement concrete
on a prepared subgrade. The Contractor shall furnish all labor, materials and equipment necessary for the
construction of the pavement in accordance with these specifications and in reasonably close conformity
to the lines, grades, thicknesses and details indicated by the plans or as established by the Engineer. All
tests shall be performed by a laboratory approved by the Engineer.
Reinforcing steel for concrete shall be deformed billet-steel bars conforming to the requirements for
Grade 40 in the latest revision of Standard Specification for Deformed Billet Steel Bars for Concrete
Reinforcement (ASTM A-615). The supplier shall certify in writing that the reinforcing steel meets the
required chemical and physical properties. The City reserves the right to sample and test reinforcing bars
after arrival at the construction site to verify the supplier's certification. Such test samples shall be
duplicate bars not less than 36 inches in length and bars from which such samples are obtained shall be
replaced at the Contractor's expense. All reinforcement bars shall be cut and bent in the fabricating shop
before shipment to the project, unless otherwise authorized by the Engineer. All reinforcement bars shall
be bent cold. All reinforcement bars or steel shall be free from detrimental dirt, scale, grease, oil, fins,
tears, excessive rust, or any other foreign substance.
Welded steel wire fabric used as reinforcement for concrete shall conform to the latest revision of ASTM
A-185. Gages, spacing and arrangement of wires and dimensions of units in flat sheet form or rolls shall
conform to the requirements as specified by the plans or contract. The supplier shall certify in writing that
the welded steel wire fabric meets the required chemical and physical properties. The City reserves the
right to sample and test welded wire fabric after arrival at the construction site to verify the supplier's
certification. All welded steel wire fabric shall be free from detrimental dirt, scale, grease, oil, fins, tears,
excessive rust or any other foreign substance.
In lieu of welded wire reinforcement, concrete shall contain polypropylene fibers thoroughly
blended into the mixture at the rate recommended by the manufacturer or as specified by the
Engineer when special properties are required. The fibers shall be "Fibermesh", "Grace Fibers" or
an approved equal. Fiberized concrete shall conform to the fiber manufacturer's specifications.
The synthetic fibers shall be manufactured from 100% virgin polypropylene in collated, fibrillated
form and shall be alkali resistant, non-absorptive and completely non-corrosive.
Fibers shall comply with ASTM C-1116, 4.1.3, Type III for durability and ASTM C-116,
Performance Level 1, I>5 as outlined in Section 21 for toughness. Certification of compliance shall
be made available upon request. Standard ACI 302 procedures for placing, finishing, and curing
shall be followed.
c) Mix Requirements
Fibers may be added to concrete at any point during the batching or mixing process. Fibers may
be added to the aggregate during weighing or charging, or to the central mixer or truck before,
during, or after charging. The load must be mixed at high speed for five minutes, or 70
revolutions, after the addition of the fibers to insure uniform distribution.
Cement shall meet the requirements of the standard specifications for Portland Cement, ASTM C150,
except that the total alkalies (no. >20+(0.638xK20)) shall not exceed 0.60 percent. Type II cement shall
have a sum of tricalcium silicate and tricalcium aluminate not exceeding 58.0 percent and the percentage
of tricalcium silicate shall not be less than 40 percent in addition to the preceeding requirements. Type I
cement may be used for all concrete work. Type II cement may be used only when approved by the
Engineer. Cement of different types shall not be mixed during storage or used alternately in any one part
of a structure. Cement shall be stored in railroad cars or in other suitable moisture-proof storage. Caked
or reclaimed cement shall not be used. The cement supplier and the concrete producer shall certify in
writing that the cement used conforms to the required chemical and physical properties. The City reserves
the right to sample the cement at the concrete production site and to test it to verify the certification.
Fine aggregate to be used in concrete shall consist of natural sand resulting from the disintegration of
siliceous and/or calcareous rocks and manufactured sand produced by crushing predominantly siliceous
materials and shall be uniformly graded from coarse to fine. This type of aggregate shall be free from
injurious amounts of organic impurities and from injurious amounts of alkali. Other deleterious substances
shall not exceed the following percentages by weight:
Material passing No. 200 sieve 2.0
Shale, lignite, coal, soft or flaky fragments 1.0
Sticks (wet) 0.1
Clay lumps (wet, on No. 4 sieve) 0.25
Fine aggregate shall meet the following gradation requirements when tested as specified by ASTM
Method C 136:
Retained on 3/8 inch sieve 0%
Retained on No. 4 sieve 0%-5%
Retained on No. 8 sieve 0%-20%
Retained on No. 16 sieve 15%-50%
Retained on No. 30 sieve 40%-75%
Retained on No. 50 sieve 70%-95%
Retained on No. 100 sieve 90%-100%
The fine aggregate shall also have a fineness modulus of not less than 2.50 or more than 3.40 and the
percent retained between any two consecutive sieves shall not be more than twenty-five percent (25%).
Fine aggregates produced or handled by hydraulic methods, and washed aggregates, shall be stockpiled
or binned for draining at least 24 hours prior to being used to produce concrete. The City reserves the
right to sample fine aggregate at the concrete production site and to conduct tests to verify that the
aggregate meets the specified requirements.
Coarse aggregate to be used in concrete shall consist of gravel, crushed gravel, crushed ston